# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2020

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_rrr
_database_code_depnum_ccdc_archive 'CCDC 1966015'
_audit_update_record             
;
2019-11-15 deposited with the CCDC.	2020-02-13 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2013
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'B19 Ba24 O57 Rb9'
_chemical_formula_weight         5182.78

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      trigonal
_space_group_IT_number           164
_space_group_name_H-M_alt        'P -3 m 1'
_space_group_name_Hall           '-P 3 2"'

_shelx_space_group_comment       
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'

_cell_length_a                   16.977(3)
_cell_length_b                   16.977(3)
_cell_length_c                   7.282(2)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     1817.7(8)
_cell_formula_units_Z            1
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    2186
_cell_measurement_theta_min      2.40
_cell_measurement_theta_max      26.41

_exptl_crystal_description       block
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      4.735
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.735
_exptl_crystal_F_000             2228
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.145
_exptl_crystal_size_mid          0.136
_exptl_crystal_size_min          0.125
_exptl_absorpt_coefficient_mu    18.841
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   none
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            11359
_diffrn_reflns_av_unetI/netI     0.0354
_diffrn_reflns_av_R_equivalents  0.0607
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_theta_min         2.399
_diffrn_reflns_theta_max         27.461
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_point_group_measured_fraction_full 0.998
_reflns_number_total             1531
_reflns_number_gt                1309
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
; 
 Reflections were merged by SHELXL according to the crystal 
 class for the calculation of statistics and refinement. 
  
 _reflns_Friedel_fraction is defined as the number of unique 
 Friedel pairs measured divided by the number that would be 
 possible theoretically, ignoring centric projections and 
 systematic absences. 
;

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 ? 
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
; 
 w=1/[σ²(Fo²)+(0.0251P)²+12.3313P] 
 where P=(Fo²+2Fc²)/3 
;
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00272(10)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         1531
_refine_ls_number_parameters     106
_refine_ls_number_restraints     6
_refine_ls_R_factor_all          0.0355
_refine_ls_R_factor_gt           0.0270
_refine_ls_wR_factor_ref         0.0633
_refine_ls_wR_factor_gt          0.0605
_refine_ls_goodness_of_fit_ref   1.043
_refine_ls_restrained_S_all      1.041
_refine_ls_shift/su_max          0.031
_refine_ls_shift/su_mean         0.001

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O 0.2633(3) 0.5266(5) 0.3643(11) 0.0271(18) Uani 1 2 d S T P . .
O2 O 0.2703(3) 0.3999(3) 0.2405(6) 0.0134(10) Uani 1 1 d . . . . .
B1 B 0.2216(4) 0.4433(7) 0.2833(14) 0.010(2) Uani 1 2 d S T P . .
O3 O 0.4647(3) 0.3952(3) 0.3118(6) 0.0156(10) Uani 1 1 d . . . . .
O4 O 0.5604(3) 0.4396(3) 0.0422(9) 0.0216(16) Uani 1 2 d S T P . .
B2 B 0.5443(4) 0.4557(4) 0.2189(14) 0.010(2) Uani 1 2 d S T P . .
O5 O 0.2644(3) 0.2026(3) 0.1806(6) 0.0154(10) Uani 1 1 d . . . . .
O6 O 0.2412(5) 0.1206(3) 0.4621(8) 0.0204(16) Uani 1 2 d S T P . .
B3 B 0.2532(7) 0.1266(4) 0.2757(15) 0.013(2) Uani 1 2 d S T P . .
Ba1 Ba 0.43751(2) 0.56249(2) 0.35393(7) 0.01178(15) Uani 1 2 d S T P . .
Ba2 Ba 0.30324(3) 0.30324(3) 0.5000 0.00930(15) Uani 1 2 d S T P . .
Ba3 Ba 0.0000 0.36445(3) 0.0000 0.01013(15) Uani 1 2 d S T P . .
Ba4 Ba 0.11298(2) 0.22595(4) 0.15776(8) 0.01584(16) Uani 1 2 d S T P . .
Rb1 Rb 0.0000 0.0000 0.5000 0.0898(17) Uani 1 12 d S T P . .
Rb2 Rb 0.46683(8) 0.23341(4) 0.2062(2) 0.0364(3) Uani 1 2 d S T P . .
Rb3 Rb 0.3333 0.6667 0.0905(3) 0.0394(5) Uani 1 6 d S T P . .
O7 O 0.0712(17) 0.0356(9) 0.108(4) 0.106(10) Uani 0.5 2 d S T P . .
B4 B 0.0000 0.0000 0.0000 0.04031(13) Uani 1 12 d S TU P . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O1 B1 1.360(13) . ?
O1 Ba1 2.7059(17) 3_565 ?
O1 Ba1 2.7060(16) . ?
O1 Rb3 2.866(8) . ?
O1 Rb2 3.249(8) 9_556 ?
O2 B1 1.388(7) . ?
O2 Ba3 2.636(4) 8 ?
O2 Ba2 2.738(5) . ?
O2 Ba4 2.886(5) . ?
O2 Ba1 2.920(4) . ?
O2 Rb2 3.602(5) 9 ?
B1 O2 1.388(7) 11 ?
B1 Ba1 3.221(6) 3_565 ?
B1 Rb2 3.581(10) 9 ?
B1 Rb2 3.734(10) 9_556 ?
O3 B2 1.396(7) . ?
O3 Ba3 2.727(4) 8 ?
O3 Ba2 2.749(5) . ?
O3 Ba1 2.829(4) 7_666 ?
O3 Rb2 2.870(5) . ?
O3 Ba1 3.112(5) . ?
O4 B2 1.371(12) . ?
O4 Ba1 2.886(6) 7_665 ?
O4 Ba3 2.923(5) 8 ?
O4 Ba3 2.923(5) 2_665 ?
O4 Rb2 3.263(5) 3_665 ?
O4 Rb2 3.263(5) . ?
O4 Rb3 3.271(7) 7_665 ?
B2 O3 1.396(7) 10_665 ?
B2 Ba3 3.087(7) 8 ?
B2 Ba3 3.087(7) 2_665 ?
B2 Ba1 3.157(10) 7_666 ?
B2 Rb2 3.320(7) 3_665 ?
O5 B3 1.391(7) . ?
O5 Ba3 2.738(5) 8 ?
O5 Ba2 2.764(4) . ?
O5 Ba4 2.796(5) . ?
O5 Ba4 2.796(5) 8 ?
O5 Rb2 3.212(5) . ?
O6 B3 1.369(12) . ?
O6 Ba2 2.745(3) . ?
O6 Ba2 2.745(3) 8_556 ?
O6 Ba4 2.777(6) 8_556 ?
O6 Rb1 3.557(8) . ?
B3 O5 1.391(7) 12 ?
B3 Ba2 3.136(6) 8_556 ?
B3 Ba4 3.182(11) 8 ?
Ba1 O1 2.7059(16) 2_665 ?
Ba1 O3 2.829(4) 7_666 ?
Ba1 O3 2.829(4) 4_556 ?
Ba1 O4 2.886(6) 7_665 ?
Ba1 O2 2.920(4) 10_665 ?
Ba1 O3 3.112(5) 10_665 ?
Ba1 B2 3.157(10) 7_666 ?
Ba1 B1 3.221(6) 2_665 ?
Ba1 Ba3 3.9135(9) 8 ?
Ba2 O2 2.738(5) 4_556 ?
Ba2 O6 2.745(3) 9_556 ?
Ba2 O3 2.749(5) 4_556 ?
Ba2 O5 2.764(4) 4_556 ?
Ba2 B3 3.136(6) 9_556 ?
Ba2 Ba4 3.7588(8) . ?
Ba2 Ba4 3.7588(8) 8_556 ?
Ba2 Ba3 3.7866(12) 8_556 ?
Ba3 O2 2.636(4) 9 ?
Ba3 O2 2.636(4) 11 ?
Ba3 O3 2.727(4) 11 ?
Ba3 O3 2.727(4) 9 ?
Ba3 O5 2.738(5) 9 ?
Ba3 O5 2.738(5) 11 ?
Ba3 O4 2.923(5) 9 ?
Ba3 O4 2.923(5) 3_565 ?
Ba3 B2 3.087(7) 3_565 ?
Ba3 B2 3.087(7) 9 ?
Ba3 Rb2 3.7539(9) 2 ?
Ba3 Rb2 3.7538(10) 9 ?
Ba4 O6 2.777(6) 9_556 ?
Ba4 O5 2.796(5) 11 ?
Ba4 O5 2.796(5) 4 ?
Ba4 O5 2.796(5) 9 ?
Ba4 O2 2.886(5) 11 ?
Ba4 O7 2.964(6) . ?
Ba4 O7 2.964(6) 2 ?
Ba4 O7 2.98(3) 9 ?
Ba4 B3 3.182(11) 9 ?
Rb1 O7 3.04(3) 8_556 ?
Rb1 O7 3.04(3) 2 ?
Rb1 O7 3.04(3) 3 ?
Rb1 O7 3.04(3) 9_556 ?
Rb1 O7 3.04(3) . ?
Rb1 O7 3.04(3) 7_556 ?
Rb1 O6 3.557(8) 9_556 ?
Rb1 O6 3.557(8) 3 ?
Rb1 O6 3.557(8) 7_556 ?
Rb1 O6 3.557(8) 8_556 ?
Rb1 O6 3.557(8) 2 ?
Rb2 O3 2.870(5) 12 ?
Rb2 O5 3.212(5) 12 ?
Rb2 O1 3.249(8) 8_556 ?
Rb2 O4 3.263(5) 2_655 ?
Rb2 B2 3.320(7) 2_655 ?
Rb2 B1 3.581(10) 8 ?
Rb2 O2 3.602(5) 8 ?
Rb2 O2 3.602(5) 4 ?
Rb2 Rb3 3.6472(19) 7_665 ?
Rb3 O1 2.866(8) 3_565 ?
Rb3 O1 2.866(8) 2_665 ?
Rb3 O4 3.271(7) 9 ?
Rb3 O4 3.271(7) 8_565 ?
Rb3 O4 3.271(7) 7_665 ?
Rb3 B1 3.572(10) 3_565 ?
Rb3 B1 3.572(10) 2_665 ?
Rb3 Ba1 3.6145(14) 2_665 ?
Rb3 Ba1 3.6145(14) 3_565 ?
Rb3 Rb2 3.6472(19) 8_565 ?
Rb3 Rb2 3.6472(19) 9 ?
O7 B4 1.31(3) . ?
O7 O7 1.81(4) 2 ?
O7 O7 1.81(4) 3 ?
O7 Ba4 2.964(6) 3 ?
O7 Ba4 2.98(3) 8 ?
B4 O7 1.31(3) 8 ?
B4 O7 1.31(3) 2 ?
B4 O7 1.31(3) 7 ?
B4 O7 1.31(3) 3 ?
B4 O7 1.31(3) 9 ?
B4 Rb1 3.6412(12) 1_554 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
B1 O1 Ba1 99.40(16) . 3_565 ?
B1 O1 Ba1 99.40(16) . . ?
Ba1 O1 Ba1 157.3(3) 3_565 . ?
B1 O1 Rb3 110.2(6) . . ?
Ba1 O1 Rb3 80.82(17) 3_565 . ?
Ba1 O1 Rb3 80.82(17) . . ?
B1 O1 Rb2 100.0(6) . 9_556 ?
Ba1 O1 Rb2 94.57(17) 3_565 9_556 ?
Ba1 O1 Rb2 94.57(17) . 9_556 ?
Rb3 O1 Rb2 149.8(3) . 9_556 ?
B1 O2 Ba3 149.3(5) . 8 ?
B1 O2 Ba2 121.1(5) . . ?
Ba3 O2 Ba2 89.56(14) 8 . ?
B1 O2 Ba4 95.6(4) . . ?
Ba3 O2 Ba4 89.08(13) 8 . ?
Ba2 O2 Ba4 83.82(12) . . ?
B1 O2 Ba1 89.5(4) . . ?
Ba3 O2 Ba1 89.41(13) 8 . ?
Ba2 O2 Ba1 88.73(12) . . ?
Ba4 O2 Ba1 172.41(18) . . ?
B1 O2 Rb2 78.0(5) . 9 ?
Ba3 O2 Rb2 72.11(10) 8 9 ?
Ba2 O2 Rb2 158.76(16) . 9 ?
Ba4 O2 Rb2 85.20(11) . 9 ?
Ba1 O2 Rb2 101.40(12) . 9 ?
O1 B1 O2 120.7(4) . . ?
O1 B1 O2 120.7(4) . 11 ?
O2 B1 O2 118.6(9) . 11 ?
O1 B1 Ba1 55.98(17) . 3_565 ?
O2 B1 Ba1 173.5(6) . 3_565 ?
O2 B1 Ba1 65.0(3) 11 3_565 ?
O1 B1 Rb2 110.2(6) . 9 ?
O2 B1 Rb2 79.7(5) . 9 ?
O2 B1 Rb2 79.7(5) 11 9 ?
Ba1 B1 Rb2 96.1(2) 3_565 9 ?
O1 B1 Rb2 59.0(5) . 9_556 ?
O2 B1 Rb2 105.4(5) . 9_556 ?
O2 B1 Rb2 105.4(5) 11 9_556 ?
Ba1 B1 Rb2 77.9(2) 3_565 9_556 ?
Rb2 B1 Rb2 169.1(3) 9 9_556 ?
B2 O3 Ba3 91.1(4) . 8 ?
B2 O3 Ba2 169.4(5) . . ?
Ba3 O3 Ba2 87.50(14) 8 . ?
B2 O3 Ba1 90.1(4) . 7_666 ?
Ba3 O3 Ba1 174.7(2) 8 7_666 ?
Ba2 O3 Ba1 90.40(13) . 7_666 ?
B2 O3 Rb2 96.0(5) . . ?
Ba3 O3 Rb2 84.20(13) 8 . ?
Ba2 O3 Rb2 94.35(14) . . ?
Ba1 O3 Rb2 100.78(15) 7_666 . ?
B2 O3 Ba1 84.7(5) . . ?
Ba3 O3 Ba1 83.89(13) 8 . ?
Ba2 O3 Ba1 84.73(13) . . ?
Ba1 O3 Ba1 91.11(13) 7_666 . ?
Rb2 O3 Ba1 168.08(17) . . ?
B2 O4 Ba1 161.0(6) . 7_665 ?
B2 O4 Ba3 83.6(4) . 8 ?
Ba1 O4 Ba3 84.72(16) 7_665 8 ?
B2 O4 Ba3 83.6(4) . 2_665 ?
Ba1 O4 Ba3 84.72(16) 7_665 2_665 ?
Ba3 O4 Ba3 103.9(2) 8 2_665 ?
B2 O4 Rb2 80.3(3) . 3_665 ?
Ba1 O4 Rb2 110.80(15) 7_665 3_665 ?
Ba3 O4 Rb2 163.9(2) 8 3_665 ?
Ba3 O4 Rb2 74.50(4) 2_665 3_665 ?
B2 O4 Rb2 80.3(3) . . ?
Ba1 O4 Rb2 110.80(15) 7_665 . ?
Ba3 O4 Rb2 74.50(4) 8 . ?
Ba3 O4 Rb2 163.9(2) 2_665 . ?
Rb2 O4 Rb2 102.5(2) 3_665 . ?
B2 O4 Rb3 127.4(6) . 7_665 ?
Ba1 O4 Rb3 71.59(15) 7_665 7_665 ?
Ba3 O4 Rb3 123.32(13) 8 7_665 ?
Ba3 O4 Rb3 123.32(13) 2_665 7_665 ?
Rb2 O4 Rb3 67.86(13) 3_665 7_665 ?
Rb2 O4 Rb3 67.86(13) . 7_665 ?
O4 B2 O3 121.6(4) . . ?
O4 B2 O3 121.6(4) . 10_665 ?
O3 B2 O3 116.7(8) . 10_665 ?
O4 B2 Ba3 70.2(3) . 8 ?
O3 B2 Ba3 62.0(3) . 8 ?
O3 B2 Ba3 143.2(6) 10_665 8 ?
O4 B2 Ba3 70.2(3) . 2_665 ?
O3 B2 Ba3 143.2(6) . 2_665 ?
O3 B2 Ba3 62.0(3) 10_665 2_665 ?
Ba3 B2 Ba3 96.4(3) 8 2_665 ?
O4 B2 Ba1 150.0(7) . 7_666 ?
O3 B2 Ba1 63.7(4) . 7_666 ?
O3 B2 Ba1 63.7(4) 10_665 7_666 ?
Ba3 B2 Ba1 125.47(19) 8 7_666 ?
Ba3 B2 Ba1 125.47(19) 2_665 7_666 ?
O4 B2 Rb2 75.7(4) . 3_665 ?
O3 B2 Rb2 142.6(6) . 3_665 ?
O3 B2 Rb2 59.3(3) 10_665 3_665 ?
Ba3 B2 Rb2 145.9(3) 8 3_665 ?
Ba3 B2 Rb2 71.63(8) 2_665 3_665 ?
Ba1 B2 Rb2 85.3(2) 7_666 3_665 ?
B3 O5 Ba3 153.9(5) . 8 ?
B3 O5 Ba2 91.9(4) . . ?
Ba3 O5 Ba2 86.99(14) 8 . ?
B3 O5 Ba4 116.9(5) . . ?
Ba3 O5 Ba4 88.97(13) 8 . ?
Ba2 O5 Ba4 85.08(12) . . ?
B3 O5 Ba4 92.7(4) . 8 ?
Ba3 O5 Ba4 88.95(13) 8 8 ?
Ba2 O5 Ba4 175.31(18) . 8 ?
Ba4 O5 Ba4 92.50(14) . 8 ?
B3 O5 Rb2 76.2(5) . . ?
Ba3 O5 Rb2 77.78(12) 8 . ?
Ba2 O5 Rb2 86.88(13) . . ?
Ba4 O5 Rb2 164.84(18) . . ?
Ba4 O5 Rb2 94.56(13) 8 . ?
B3 O6 Ba2 93.2(2) . . ?
B3 O6 Ba2 93.2(2) . 8_556 ?
Ba2 O6 Ba2 139.4(3) . 8_556 ?
B3 O6 Ba4 177.2(7) . 8_556 ?
Ba2 O6 Ba4 85.79(14) . 8_556 ?
Ba2 O6 Ba4 85.79(14) 8_556 8_556 ?
B3 O6 Rb1 101.9(6) . . ?
Ba2 O6 Rb1 108.88(15) . . ?
Ba2 O6 Rb1 108.88(15) 8_556 . ?
Ba4 O6 Rb1 80.92(17) 8_556 . ?
O6 B3 O5 120.6(4) . . ?
O6 B3 O5 120.6(4) . 12 ?
O5 B3 O5 118.4(8) . 12 ?
O6 B3 Ba2 60.9(2) . 8_556 ?
O5 B3 Ba2 159.5(7) . 8_556 ?
O5 B3 Ba2 61.7(3) 12 8_556 ?
O6 B3 Ba4 165.3(7) . 8 ?
O5 B3 Ba4 61.4(4) . 8 ?
O5 B3 Ba4 61.4(4) 12 8 ?
Ba2 B3 Ba4 123.11(17) 8_556 8 ?
O1 Ba1 O1 82.4(3) 2_665 . ?
O1 Ba1 O3 85.2(2) 2_665 7_666 ?
O1 Ba1 O3 117.99(19) . 7_666 ?
O1 Ba1 O3 117.99(19) 2_665 4_556 ?
O1 Ba1 O3 85.2(2) . 4_556 ?
O3 Ba1 O3 49.68(19) 7_666 4_556 ?
O1 Ba1 O4 92.5(2) 2_665 7_665 ?
O1 Ba1 O4 92.5(2) . 7_665 ?
O3 Ba1 O4 148.66(13) 7_666 7_665 ?
O3 Ba1 O4 148.66(13) 4_556 7_665 ?
O1 Ba1 O2 50.08(17) 2_665 10_665 ?
O1 Ba1 O2 128.46(19) . 10_665 ?
O3 Ba1 O2 81.22(13) 7_666 10_665 ?
O3 Ba1 O2 130.78(13) 4_556 10_665 ?
O4 Ba1 O2 73.60(8) 7_665 10_665 ?
O1 Ba1 O2 128.47(19) 2_665 . ?
O1 Ba1 O2 50.08(17) . . ?
O3 Ba1 O2 130.78(13) 7_666 . ?
O3 Ba1 O2 81.22(13) 4_556 . ?
O4 Ba1 O2 73.60(8) 7_665 . ?
O2 Ba1 O2 147.01(17) 10_665 . ?
O1 Ba1 O3 160.93(18) 2_665 . ?
O1 Ba1 O3 116.22(18) . . ?
O3 Ba1 O3 88.89(13) 7_666 . ?
O3 Ba1 O3 70.10(15) 4_556 . ?
O4 Ba1 O3 83.20(16) 7_665 . ?
O2 Ba1 O3 111.10(12) 10_665 . ?
O2 Ba1 O3 68.13(12) . . ?
O1 Ba1 O3 116.21(18) 2_665 10_665 ?
O1 Ba1 O3 160.93(18) . 10_665 ?
O3 Ba1 O3 70.10(15) 7_666 10_665 ?
O3 Ba1 O3 88.89(13) 4_556 10_665 ?
O4 Ba1 O3 83.20(16) 7_665 10_665 ?
O2 Ba1 O3 68.13(12) 10_665 10_665 ?
O2 Ba1 O3 111.10(12) . 10_665 ?
O3 Ba1 O3 44.91(17) . 10_665 ?
O1 Ba1 B2 95.7(2) 2_665 7_666 ?
O1 Ba1 B2 95.7(2) . 7_666 ?
O3 Ba1 B2 26.25(11) 7_666 7_666 ?
O3 Ba1 B2 26.24(11) 4_556 7_666 ?
O4 Ba1 B2 169.0(2) 7_665 7_666 ?
O2 Ba1 B2 106.43(8) 10_665 7_666 ?
O2 Ba1 B2 106.43(8) . 7_666 ?
O3 Ba1 B2 86.64(19) . 7_666 ?
O3 Ba1 B2 86.64(19) 10_665 7_666 ?
O1 Ba1 B1 24.6(2) 2_665 2_665 ?
O1 Ba1 B1 104.8(2) . 2_665 ?
O3 Ba1 B1 83.9(2) 7_666 2_665 ?
O3 Ba1 B1 129.5(2) 4_556 2_665 ?
O4 Ba1 B1 81.36(19) 7_665 2_665 ?
O2 Ba1 B1 25.53(18) 10_665 2_665 ?
O2 Ba1 B1 142.29(19) . 2_665 ?
O3 Ba1 B1 136.63(18) . 2_665 ?
O3 Ba1 B1 93.00(18) 10_665 2_665 ?
B2 Ba1 B1 103.4(2) 7_666 2_665 ?
O1 Ba1 Ba3 139.36(17) 2_665 8 ?
O1 Ba1 Ba3 89.07(15) . 8 ?
O3 Ba1 Ba3 132.73(10) 7_666 8 ?
O3 Ba1 Ba3 100.63(10) 4_556 8 ?
O4 Ba1 Ba3 48.05(9) 7_665 8 ?
O2 Ba1 Ba3 112.87(9) 10_665 8 ?
O2 Ba1 Ba3 42.35(8) . 8 ?
O3 Ba1 Ba3 43.86(8) . 8 ?
O3 Ba1 Ba3 74.23(8) 10_665 8 ?
B2 Ba1 Ba3 124.71(13) 7_666 8 ?
B1 Ba1 Ba3 128.40(18) 2_665 8 ?
O2 Ba2 O2 157.21(19) . 4_556 ?
O2 Ba2 O6 76.66(17) . 9_556 ?
O2 Ba2 O6 122.00(16) 4_556 9_556 ?
O2 Ba2 O6 122.00(16) . . ?
O2 Ba2 O6 76.66(17) 4_556 . ?
O6 Ba2 O6 81.7(3) 9_556 . ?
O2 Ba2 O3 86.02(13) . 4_556 ?
O2 Ba2 O3 76.11(13) 4_556 4_556 ?
O6 Ba2 O3 107.58(18) 9_556 4_556 ?
O6 Ba2 O3 151.98(16) . 4_556 ?
O2 Ba2 O3 76.11(13) . . ?
O2 Ba2 O3 86.02(13) 4_556 . ?
O6 Ba2 O3 151.98(16) 9_556 . ?
O6 Ba2 O3 107.58(18) . . ?
O3 Ba2 O3 76.94(19) 4_556 . ?
O2 Ba2 O5 74.50(13) . . ?
O2 Ba2 O5 115.88(13) 4_556 . ?
O6 Ba2 O5 88.45(17) 9_556 . ?
O6 Ba2 O5 51.60(15) . . ?
O3 Ba2 O5 151.33(14) 4_556 . ?
O3 Ba2 O5 78.07(14) . . ?
O2 Ba2 O5 115.88(13) . 4_556 ?
O2 Ba2 O5 74.50(13) 4_556 4_556 ?
O6 Ba2 O5 51.60(16) 9_556 4_556 ?
O6 Ba2 O5 88.46(17) . 4_556 ?
O3 Ba2 O5 78.06(14) 4_556 4_556 ?
O3 Ba2 O5 151.33(14) . 4_556 ?
O5 Ba2 O5 129.3(2) . 4_556 ?
O2 Ba2 B3 93.86(19) . 9_556 ?
O2 Ba2 B3 100.08(19) 4_556 9_556 ?
O6 Ba2 B3 25.8(2) 9_556 9_556 ?
O6 Ba2 B3 88.4(2) . 9_556 ?
O3 Ba2 B3 90.0(2) 4_556 9_556 ?
O3 Ba2 B3 163.9(2) . 9_556 ?
O5 Ba2 B3 111.8(2) . 9_556 ?
O5 Ba2 B3 26.32(19) 4_556 9_556 ?
O2 Ba2 Ba4 49.77(9) . . ?
O2 Ba2 Ba4 152.21(9) 4_556 . ?
O6 Ba2 Ba4 47.47(13) 9_556 . ?
O6 Ba2 Ba4 76.21(14) . . ?
O3 Ba2 Ba4 129.75(10) 4_556 . ?
O3 Ba2 Ba4 107.86(9) . . ?
O5 Ba2 Ba4 47.82(10) . . ?
O5 Ba2 Ba4 98.86(10) 4_556 . ?
B3 Ba2 Ba4 73.28(17) 9_556 . ?
O2 Ba2 Ba4 152.21(9) . 8_556 ?
O2 Ba2 Ba4 49.77(9) 4_556 8_556 ?
O6 Ba2 Ba4 76.21(14) 9_556 8_556 ?
O6 Ba2 Ba4 47.47(13) . 8_556 ?
O3 Ba2 Ba4 107.86(9) 4_556 8_556 ?
O3 Ba2 Ba4 129.75(10) . 8_556 ?
O5 Ba2 Ba4 98.86(10) . 8_556 ?
O5 Ba2 Ba4 47.82(10) 4_556 8_556 ?
B3 Ba2 Ba4 63.02(17) 9_556 8_556 ?
Ba4 Ba2 Ba4 105.66(3) . 8_556 ?
O2 Ba2 Ba3 127.55(9) . 8_556 ?
O2 Ba2 Ba3 44.12(9) 4_556 8_556 ?
O6 Ba2 Ba3 96.37(13) 9_556 8_556 ?
O6 Ba2 Ba3 107.72(13) . 8_556 ?
O3 Ba2 Ba3 46.01(9) 4_556 8_556 ?
O3 Ba2 Ba3 105.35(9) . 8_556 ?
O5 Ba2 Ba3 157.95(9) . 8_556 ?
O5 Ba2 Ba3 46.23(10) 4_556 8_556 ?
B3 Ba2 Ba3 70.58(18) 9_556 8_556 ?
Ba4 Ba2 Ba3 143.458(13) . 8_556 ?
Ba4 Ba2 Ba3 61.850(18) 8_556 8_556 ?
O2 Ba3 O2 158.2(2) 9 11 ?
O2 Ba3 O3 111.05(14) 9 11 ?
O2 Ba3 O3 78.17(14) 11 11 ?
O2 Ba3 O3 78.17(14) 9 9 ?
O2 Ba3 O3 111.05(14) 11 9 ?
O3 Ba3 O3 131.84(19) 11 9 ?
O2 Ba3 O5 76.56(14) 9 9 ?
O2 Ba3 O5 85.74(13) 11 9 ?
O3 Ba3 O5 148.82(13) 11 9 ?
O3 Ba3 O5 78.87(14) 9 9 ?
O2 Ba3 O5 85.74(13) 9 11 ?
O2 Ba3 O5 76.56(14) 11 11 ?
O3 Ba3 O5 78.87(14) 11 11 ?
O3 Ba3 O5 148.82(13) 9 11 ?
O5 Ba3 O5 71.5(2) 9 11 ?
O2 Ba3 O4 121.21(16) 9 9 ?
O2 Ba3 O4 77.25(15) 11 9 ?
O3 Ba3 O4 89.66(16) 11 9 ?
O3 Ba3 O4 50.47(16) 9 9 ?
O5 Ba3 O4 112.77(16) 9 9 ?
O5 Ba3 O4 153.05(15) 11 9 ?
O2 Ba3 O4 77.25(15) 9 3_565 ?
O2 Ba3 O4 121.21(16) 11 3_565 ?
O3 Ba3 O4 50.47(16) 11 3_565 ?
O3 Ba3 O4 89.66(16) 9 3_565 ?
O5 Ba3 O4 153.05(15) 9 3_565 ?
O5 Ba3 O4 112.77(16) 11 3_565 ?
O4 Ba3 O4 76.1(2) 9 3_565 ?
O2 Ba3 B2 100.3(2) 9 3_565 ?
O2 Ba3 B2 95.9(2) 11 3_565 ?
O3 Ba3 B2 26.88(17) 11 3_565 ?
O3 Ba3 B2 106.48(17) 9 3_565 ?
O5 Ba3 B2 173.28(18) 9 3_565 ?
O5 Ba3 B2 102.54(17) 11 3_565 ?
O4 Ba3 B2 73.95(19) 9 3_565 ?
O4 Ba3 B2 26.2(2) 3_565 3_565 ?
O2 Ba3 B2 95.9(2) 9 9 ?
O2 Ba3 B2 100.3(2) 11 9 ?
O3 Ba3 B2 106.48(17) 11 9 ?
O3 Ba3 B2 26.88(17) 9 9 ?
O5 Ba3 B2 102.54(17) 9 9 ?
O5 Ba3 B2 173.28(18) 11 9 ?
O4 Ba3 B2 26.2(2) 9 9 ?
O4 Ba3 B2 73.95(19) 3_565 9 ?
B2 Ba3 B2 83.6(3) 3_565 9 ?
O2 Ba3 Rb2 65.95(10) 9 2 ?
O2 Ba3 Rb2 112.52(10) 11 2 ?
O3 Ba3 Rb2 49.52(10) 11 2 ?
O3 Ba3 Rb2 134.60(10) 9 2 ?
O5 Ba3 Rb2 116.30(10) 9 2 ?
O5 Ba3 Rb2 56.75(10) 11 2 ?
O4 Ba3 Rb2 130.42(12) 9 2 ?
O4 Ba3 Rb2 56.88(12) 3_565 2 ?
B2 Ba3 Rb2 57.06(16) 3_565 2 ?
B2 Ba3 Rb2 129.82(16) 9 2 ?
O2 Ba3 Rb2 112.52(10) 9 9 ?
O2 Ba3 Rb2 65.95(10) 11 9 ?
O3 Ba3 Rb2 134.60(10) 11 9 ?
O3 Ba3 Rb2 49.52(10) 9 9 ?
O5 Ba3 Rb2 56.75(10) 9 9 ?
O5 Ba3 Rb2 116.30(10) 11 9 ?
O4 Ba3 Rb2 56.88(12) 9 9 ?
O4 Ba3 Rb2 130.42(12) 3_565 9 ?
B2 Ba3 Rb2 129.82(16) 3_565 9 ?
B2 Ba3 Rb2 57.06(16) 9 9 ?
Rb2 Ba3 Rb2 172.57(4) 2 9 ?
O6 Ba4 O5 87.17(9) 9_556 11 ?
O6 Ba4 O5 87.17(9) 9_556 . ?
O5 Ba4 O5 164.32(19) 11 . ?
O6 Ba4 O5 149.54(13) 9_556 4 ?
O5 Ba4 O5 120.04(9) 11 4 ?
O5 Ba4 O5 69.75(15) . 4 ?
O6 Ba4 O5 149.54(13) 9_556 9 ?
O5 Ba4 O5 69.75(15) 11 9 ?
O5 Ba4 O5 120.04(9) . 9 ?
O5 Ba4 O5 50.60(18) 4 9 ?
O6 Ba4 O2 73.76(17) 9_556 . ?
O5 Ba4 O2 120.40(13) 11 . ?
O5 Ba4 O2 71.74(13) . . ?
O5 Ba4 O2 80.09(13) 4 . ?
O5 Ba4 O2 100.45(13) 9 . ?
O6 Ba4 O2 73.76(17) 9_556 11 ?
O5 Ba4 O2 71.74(13) 11 11 ?
O5 Ba4 O2 120.40(13) . 11 ?
O5 Ba4 O2 100.45(13) 4 11 ?
O5 Ba4 O2 80.09(13) 9 11 ?
O2 Ba4 O2 48.85(18) . 11 ?
O6 Ba4 O7 101.5(6) 9_556 . ?
O5 Ba4 O7 101.2(5) 11 . ?
O5 Ba4 O7 65.7(5) . . ?
O5 Ba4 O7 87.2(6) 4 . ?
O5 Ba4 O7 102.3(5) 9 . ?
O2 Ba4 O7 137.4(5) . . ?
O2 Ba4 O7 171.4(6) 11 . ?
O6 Ba4 O7 101.5(6) 9_556 2 ?
O5 Ba4 O7 65.7(5) 11 2 ?
O5 Ba4 O7 101.2(5) . 2 ?
O5 Ba4 O7 102.3(5) 4 2 ?
O5 Ba4 O7 87.2(6) 9 2 ?
O2 Ba4 O7 171.4(6) . 2 ?
O2 Ba4 O7 137.4(5) 11 2 ?
O7 Ba4 O7 35.6(10) . 2 ?
O6 Ba4 O7 135.0(5) 9_556 9 ?
O5 Ba4 O7 86.84(11) 11 9 ?
O5 Ba4 O7 86.85(11) . 9 ?
O5 Ba4 O7 65.4(5) 4 9 ?
O5 Ba4 O7 65.4(5) 9 9 ?
O2 Ba4 O7 144.1(4) . 9 ?
O2 Ba4 O7 144.1(4) 11 9 ?
O7 Ba4 O7 37.0(9) . 9 ?
O7 Ba4 O7 37.0(9) 2 9 ?
O6 Ba4 B3 168.1(3) 9_556 9 ?
O5 Ba4 B3 94.27(9) 11 9 ?
O5 Ba4 B3 94.27(9) . 9 ?
O5 Ba4 B3 25.89(10) 4 9 ?
O5 Ba4 B3 25.89(10) 9 9 ?
O2 Ba4 B3 95.5(2) . 9 ?
O2 Ba4 B3 95.5(2) 11 9 ?
O7 Ba4 B3 89.8(6) . 9 ?
O7 Ba4 B3 89.8(6) 2 9 ?
O7 Ba4 B3 56.9(5) 9 9 ?
O6 Ba4 Ba2 46.74(6) 9_556 . ?
O5 Ba4 Ba2 132.54(9) 11 . ?
O5 Ba4 Ba2 47.10(9) . . ?
O5 Ba4 Ba2 103.32(9) 4 . ?
O5 Ba4 Ba2 144.66(10) 9 . ?
O2 Ba4 Ba2 46.41(9) . . ?
O2 Ba4 Ba2 82.93(9) 11 . ?
O7 Ba4 Ba2 99.1(5) . . ?
O7 Ba4 Ba2 125.2(6) 2 . ?
O7 Ba4 Ba2 131.3(2) 9 . ?
B3 Ba4 Ba2 128.29(10) 9 . ?
O7 Rb1 O7 180.0 8_556 2 ?
O7 Rb1 O7 145.3(8) 8_556 3 ?
O7 Rb1 O7 34.7(8) 2 3 ?
O7 Rb1 O7 34.7(8) 8_556 9_556 ?
O7 Rb1 O7 145.3(8) 2 9_556 ?
O7 Rb1 O7 180.0(6) 3 9_556 ?
O7 Rb1 O7 145.3(8) 8_556 . ?
O7 Rb1 O7 34.7(8) 2 . ?
O7 Rb1 O7 34.7(8) 3 . ?
O7 Rb1 O7 145.3(8) 9_556 . ?
O7 Rb1 O7 34.7(8) 8_556 7_556 ?
O7 Rb1 O7 145.3(8) 2 7_556 ?
O7 Rb1 O7 145.3(8) 3 7_556 ?
O7 Rb1 O7 34.7(8) 9_556 7_556 ?
O7 Rb1 O7 180.0 . 7_556 ?
O7 Rb1 O6 95.7(3) 8_556 9_556 ?
O7 Rb1 O6 84.3(3) 2 9_556 ?
O7 Rb1 O6 114.6(5) 3 9_556 ?
O7 Rb1 O6 65.4(5) 9_556 9_556 ?
O7 Rb1 O6 84.3(3) . 9_556 ?
O7 Rb1 O6 95.7(3) 7_556 9_556 ?
O7 Rb1 O6 84.3(3) 8_556 3 ?
O7 Rb1 O6 95.7(3) 2 3 ?
O7 Rb1 O6 65.4(5) 3 3 ?
O7 Rb1 O6 114.6(5) 9_556 3 ?
O7 Rb1 O6 95.7(3) . 3 ?
O7 Rb1 O6 84.3(3) 7_556 3 ?
O6 Rb1 O6 180.0 9_556 3 ?
O7 Rb1 O6 95.7(3) 8_556 7_556 ?
O7 Rb1 O6 84.3(3) 2 7_556 ?
O7 Rb1 O6 84.3(3) 3 7_556 ?
O7 Rb1 O6 95.7(3) 9_556 7_556 ?
O7 Rb1 O6 114.6(5) . 7_556 ?
O7 Rb1 O6 65.4(5) 7_556 7_556 ?
O6 Rb1 O6 119.40(3) 9_556 7_556 ?
O6 Rb1 O6 60.60(3) 3 7_556 ?
O7 Rb1 O6 65.4(5) 8_556 8_556 ?
O7 Rb1 O6 114.6(5) 2 8_556 ?
O7 Rb1 O6 84.3(3) 3 8_556 ?
O7 Rb1 O6 95.7(3) 9_556 8_556 ?
O7 Rb1 O6 84.3(3) . 8_556 ?
O7 Rb1 O6 95.7(3) 7_556 8_556 ?
O6 Rb1 O6 119.40(3) 9_556 8_556 ?
O6 Rb1 O6 60.60(3) 3 8_556 ?
O6 Rb1 O6 119.40(3) 7_556 8_556 ?
O7 Rb1 O6 114.6(5) 8_556 2 ?
O7 Rb1 O6 65.4(5) 2 2 ?
O7 Rb1 O6 95.7(3) 3 2 ?
O7 Rb1 O6 84.3(3) 9_556 2 ?
O7 Rb1 O6 95.7(3) . 2 ?
O7 Rb1 O6 84.3(3) 7_556 2 ?
O6 Rb1 O6 60.60(3) 9_556 2 ?
O6 Rb1 O6 119.40(3) 3 2 ?
O6 Rb1 O6 60.60(3) 7_556 2 ?
O6 Rb1 O6 180.0 8_556 2 ?
O7 Rb1 O6 84.3(3) 8_556 . ?
O7 Rb1 O6 95.7(3) 2 . ?
O7 Rb1 O6 95.7(3) 3 . ?
O7 Rb1 O6 84.3(3) 9_556 . ?
O7 Rb1 O6 65.4(5) . . ?
O7 Rb1 O6 114.6(5) 7_556 . ?
O6 Rb1 O6 60.60(3) 9_556 . ?
O6 Rb1 O6 119.40(3) 3 . ?
O6 Rb1 O6 180.00(15) 7_556 . ?
O6 Rb1 O6 60.60(3) 8_556 . ?
O6 Rb1 O6 119.40(3) 2 . ?
O3 Rb2 O3 148.90(18) 12 . ?
O3 Rb2 O5 69.34(13) 12 12 ?
O3 Rb2 O5 111.35(13) . 12 ?
O3 Rb2 O5 111.35(13) 12 . ?
O3 Rb2 O5 69.35(13) . . ?
O5 Rb2 O5 43.69(16) 12 . ?
O3 Rb2 O1 75.23(9) 12 8_556 ?
O3 Rb2 O1 75.23(9) . 8_556 ?
O5 Rb2 O1 107.85(15) 12 8_556 ?
O5 Rb2 O1 107.85(15) . 8_556 ?
O3 Rb2 O4 45.84(15) 12 2_655 ?
O3 Rb2 O4 154.39(15) . 2_655 ?
O5 Rb2 O4 93.48(14) 12 2_655 ?
O5 Rb2 O4 132.69(13) . 2_655 ?
O1 Rb2 O4 103.79(13) 8_556 2_655 ?
O3 Rb2 O4 154.39(15) 12 . ?
O3 Rb2 O4 45.84(15) . . ?
O5 Rb2 O4 132.69(13) 12 . ?
O5 Rb2 O4 93.48(14) . . ?
O1 Rb2 O4 103.79(13) 8_556 . ?
O4 Rb2 O4 112.1(2) 2_655 . ?
O3 Rb2 B2 24.72(17) 12 2_655 ?
O3 Rb2 B2 154.26(18) . 2_655 ?
O5 Rb2 B2 88.28(16) 12 2_655 ?
O5 Rb2 B2 131.97(16) . 2_655 ?
O1 Rb2 B2 83.13(18) 8_556 2_655 ?
O4 Rb2 B2 24.0(2) 2_655 2_655 ?
O4 Rb2 B2 130.13(19) . 2_655 ?
O3 Rb2 B1 105.40(9) 12 8 ?
O3 Rb2 B1 105.40(9) . 8 ?
O5 Rb2 B1 81.53(18) 12 8 ?
O5 Rb2 B1 81.53(18) . 8 ?
O1 Rb2 B1 169.8(2) 8_556 8 ?
O4 Rb2 B1 71.12(14) 2_655 8 ?
O4 Rb2 B1 71.12(14) . 8 ?
B2 Rb2 B1 93.49(18) 2_655 8 ?
O3 Rb2 O2 85.40(11) 12 8 ?
O3 Rb2 O2 123.94(12) . 8 ?
O5 Rb2 O2 64.62(11) 12 8 ?
O5 Rb2 O2 79.51(11) . 8 ?
O1 Rb2 O2 160.62(7) 8_556 8 ?
O4 Rb2 O2 60.63(12) 2_655 8 ?
O4 Rb2 O2 93.41(13) . 8 ?
B2 Rb2 O2 78.91(18) 2_655 8 ?
B1 Rb2 O2 22.29(11) 8 8 ?
O3 Rb2 O2 123.94(12) 12 4 ?
O3 Rb2 O2 85.40(11) . 4 ?
O5 Rb2 O2 79.51(11) 12 4 ?
O5 Rb2 O2 64.62(11) . 4 ?
O1 Rb2 O2 160.62(7) 8_556 4 ?
O4 Rb2 O2 93.41(13) 2_655 4 ?
O4 Rb2 O2 60.63(12) . 4 ?
B2 Rb2 O2 115.46(19) 2_655 4 ?
B1 Rb2 O2 22.29(11) 8 4 ?
O2 Rb2 O2 38.71(14) 8 4 ?
O3 Rb2 Rb3 99.63(9) 12 7_665 ?
O3 Rb2 Rb3 99.63(9) . 7_665 ?
O5 Rb2 Rb3 135.39(9) 12 7_665 ?
O5 Rb2 Rb3 135.39(9) . 7_665 ?
O1 Rb2 Rb3 110.63(14) 8_556 7_665 ?
O4 Rb2 Rb3 56.19(12) 2_655 7_665 ?
O4 Rb2 Rb3 56.18(12) . 7_665 ?
B2 Rb2 Rb3 74.94(15) 2_655 7_665 ?
B1 Rb2 Rb3 59.22(17) 8 7_665 ?
O2 Rb2 Rb3 71.63(8) 8 7_665 ?
O2 Rb2 Rb3 71.63(8) 4 7_665 ?
O1 Rb3 O1 76.9(2) 3_565 . ?
O1 Rb3 O1 76.9(2) 3_565 2_665 ?
O1 Rb3 O1 76.9(2) . 2_665 ?
O1 Rb3 O4 82.09(12) 3_565 9 ?
O1 Rb3 O4 82.09(12) . 9 ?
O1 Rb3 O4 153.10(19) 2_665 9 ?
O1 Rb3 O4 82.09(12) 3_565 8_565 ?
O1 Rb3 O4 153.10(19) . 8_565 ?
O1 Rb3 O4 82.09(12) 2_665 8_565 ?
O4 Rb3 O4 111.66(11) 9 8_565 ?
O1 Rb3 O4 153.10(19) 3_565 7_665 ?
O1 Rb3 O4 82.09(12) . 7_665 ?
O1 Rb3 O4 82.09(12) 2_665 7_665 ?
O4 Rb3 O4 111.66(11) 9 7_665 ?
O4 Rb3 O4 111.66(11) 8_565 7_665 ?
O1 Rb3 B1 20.9(2) 3_565 3_565 ?
O1 Rb3 B1 93.26(17) . 3_565 ?
O1 Rb3 B1 93.26(17) 2_665 3_565 ?
O4 Rb3 B1 71.15(10) 9 3_565 ?
O4 Rb3 B1 71.15(10) 8_565 3_565 ?
O4 Rb3 B1 174.0(2) 7_665 3_565 ?
O1 Rb3 B1 93.26(17) 3_565 2_665 ?
O1 Rb3 B1 93.26(17) . 2_665 ?
O1 Rb3 B1 20.9(2) 2_665 2_665 ?
O4 Rb3 B1 174.0(2) 9 2_665 ?
O4 Rb3 B1 71.15(10) 8_565 2_665 ?
O4 Rb3 B1 71.15(10) 7_665 2_665 ?
B1 Rb3 B1 105.6(2) 3_565 2_665 ?
O1 Rb3 Ba1 47.65(3) 3_565 2_665 ?
O1 Rb3 Ba1 103.86(15) . 2_665 ?
O1 Rb3 Ba1 47.65(3) 2_665 2_665 ?
O4 Rb3 Ba1 124.17(6) 9 2_665 ?
O4 Rb3 Ba1 49.24(12) 8_565 2_665 ?
O4 Rb3 Ba1 124.17(6) 7_665 2_665 ?
B1 Rb3 Ba1 53.26(7) 3_565 2_665 ?
B1 Rb3 Ba1 53.26(7) 2_665 2_665 ?
O1 Rb3 Ba1 47.65(3) 3_565 3_565 ?
O1 Rb3 Ba1 47.65(3) . 3_565 ?
O1 Rb3 Ba1 103.86(15) 2_665 3_565 ?
O4 Rb3 Ba1 49.24(12) 9 3_565 ?
O4 Rb3 Ba1 124.17(6) 8_565 3_565 ?
O4 Rb3 Ba1 124.17(6) 7_665 3_565 ?
B1 Rb3 Ba1 53.26(7) 3_565 3_565 ?
B1 Rb3 Ba1 124.80(18) 2_665 3_565 ?
Ba1 Rb3 Ba1 94.45(4) 2_665 3_565 ?
O1 Rb3 Rb2 80.42(15) 3_565 8_565 ?
O1 Rb3 Rb2 134.55(3) . 8_565 ?
O1 Rb3 Rb2 134.55(3) 2_665 8_565 ?
O4 Rb3 Rb2 55.95(7) 9 8_565 ?
O4 Rb3 Rb2 55.95(7) 8_565 8_565 ?
O4 Rb3 Rb2 126.48(14) 7_665 8_565 ?
B1 Rb3 Rb2 59.47(17) 3_565 8_565 ?
B1 Rb3 Rb2 127.10(8) 2_665 8_565 ?
Ba1 Rb3 Rb2 88.46(2) 2_665 8_565 ?
Ba1 Rb3 Rb2 88.46(2) 3_565 8_565 ?
O1 Rb3 Rb2 134.55(3) 3_565 9 ?
O1 Rb3 Rb2 80.41(15) . 9 ?
O1 Rb3 Rb2 134.55(3) 2_665 9 ?
O4 Rb3 Rb2 55.95(7) 9 9 ?
O4 Rb3 Rb2 126.48(14) 8_565 9 ?
O4 Rb3 Rb2 55.95(7) 7_665 9 ?
B1 Rb3 Rb2 127.10(8) 3_565 9 ?
B1 Rb3 Rb2 127.10(8) 2_665 9 ?
Ba1 Rb3 Rb2 175.72(6) 2_665 9 ?
Ba1 Rb3 Rb2 88.46(2) 3_565 9 ?
Rb2 Rb3 Rb2 88.48(5) 8_565 9 ?
B4 O7 O7 46.1(9) . 2 ?
B4 O7 O7 46.1(9) . 3 ?
O7 O7 O7 60.000(4) 2 3 ?
B4 O7 Ba4 103.9(5) . 3 ?
O7 O7 Ba4 131.6(5) 2 3 ?
O7 O7 Ba4 72.2(5) 3 3 ?
B4 O7 Ba4 103.9(5) . . ?
O7 O7 Ba4 72.2(5) 2 . ?
O7 O7 Ba4 131.7(5) 3 . ?
Ba4 O7 Ba4 152.1(9) 3 . ?
B4 O7 Ba4 102.8(15) . 8 ?
O7 O7 Ba4 131.3(4) 2 8 ?
O7 O7 Ba4 131.3(4) 3 8 ?
Ba4 O7 Ba4 85.5(6) 3 8 ?
Ba4 O7 Ba4 85.5(5) . 8 ?
B4 O7 Rb1 106.7(15) . . ?
O7 O7 Rb1 72.7(4) 2 . ?
O7 O7 Rb1 72.7(4) 3 . ?
Ba4 O7 Rb1 87.5(6) 3 . ?
Ba4 O7 Rb1 87.5(6) . . ?
Ba4 O7 Rb1 150.5(9) 8 . ?
O7 B4 O7 180(3) 8 2 ?
O7 B4 O7 92.2(19) 8 . ?
O7 B4 O7 87.8(19) 2 . ?
O7 B4 O7 87.8(19) 8 7 ?
O7 B4 O7 92.2(19) 2 7 ?
O7 B4 O7 180.0 . 7 ?
O7 B4 O7 92.2(19) 8 3 ?
O7 B4 O7 87.8(19) 2 3 ?
O7 B4 O7 87.8(19) . 3 ?
O7 B4 O7 92.2(19) 7 3 ?
O7 B4 O7 87.8(19) 8 9 ?
O7 B4 O7 92.2(19) 2 9 ?
O7 B4 O7 92.2(19) . 9 ?
O7 B4 O7 87.8(19) 7 9 ?
O7 B4 O7 180(3) 3 9 ?
O7 B4 Rb1 53.2(13) 8 1_554 ?
O7 B4 Rb1 126.8(13) 2 1_554 ?
O7 B4 Rb1 126.8(13) . 1_554 ?
O7 B4 Rb1 53.2(13) 7 1_554 ?
O7 B4 Rb1 126.8(13) 3 1_554 ?
O7 B4 Rb1 53.2(13) 9 1_554 ?

_refine_diff_density_max         1.653
_refine_diff_density_min         -2.454
_refine_diff_density_rms         0.257

_shelxl_version_number           2013-2

